Thank you for visiting nature.com. You are using a browser version with limited support for CSS. To obtain the best experience, we recommend you use a more up to date browser (or turn off compatibility mode in Internet Explorer). In the meantime, to ensure continued support, we are displaying the site without styles and JavaScript.

# Switching and extension of transmission response, based on bending metamaterials

## Abstract

The electromagnetically-induced transparency (EIT)-like effects in planar and non-planar metamaterials (MMs) were investigated for microwave (GHz) frequencies. The specific MMs used in this study consisted of a cut-wire resonator and a ring resonator, where were placed on the top and the bottom layers, respectively. A transmission window was produced, due to the interference between bright- and bright-mode coupling. Using the numerical and the experimental results, we demonstrate that the bending of MM leads to enhanced transmission and bandwidth, as well as an additional EIT-like peak. This provides an effective way of realizing the tunable devices, including the switching sensors.

## Introduction

Electromagnetically-induced transparency (EIT) is a quantum interference effect which is activated in coherent interaction between atomic ensembles1. The phenomenon gives rise to a sharp transmission window in the absorption spectrum. The EIT results in slow-light phenomena, this enhancing the nonlinearity associated with near-resonance effects and promoting a variety of applications, including nonlinear optics, quantum optical memories and slow-light devices2,3,4,5,6. However, the EIT phenomena in these atomic systems are hard to be realized experimentally owing both to the cryogenic operation temperatures, and the need for stable lasers to match the atomic transitions7. Recently, the coherent processes, leading to EIT, have been observed in MMs8. This can relax dramatically the difficulty in the experimental realization because of the room-temperature operation and of no need for external activation by pumping lasers. The MM structures reveal the EIT-like phenomena which are the result of Fano-type linear destructive interference among the artificial resonant elements9. The phenomena are obtained by the broken structural symmetry or by the near-field subwavelength-scale coupling10,11,12. The latter origin of EIT can be interpreted by the near-field coupling between a radiative bright resonator that couples strongly with the incident light, and a dark resonator that couples weakly with light13, 14. However, the EIT-like behavior also occurs without the dark-mode excitation, which is described by the interference between bright modes15. In addition, the EIT-like effect, based on the phase coupling, can be switched by adjusting the incident angle16, 17. Herein, we studied the EIT-like effect using bright- and bright-mode resonators18. Two types of resonators were fabricated at the top [a cut-wire resonator (CWR)] and the bottom [a ring resonator (RR)] of FR-4 substrate. By placing two types of resonators on the top and the bottom layers, they can have different phases. This allows us to have the classical analogue of EIT-like effect due to the phase coupling between CWR and RR, which leads to the enhanced transmission in the microwave range. To control effectively the transmission peak using two types of resonator modes, we have also investigated the bending effect at GHz frequencies in this EIT MM.

So far, only a few studies have been performed regarding this topic, which all reported simply on the planar substrates for the EIT-like effect working at GHz frequencies19,20,21. However, in our study here, we used non-planar substrate to elucidate the bending effect. The EIT-like feature could be controlled by adjusting the bending parameters of sample. This response tuning via bending the MM is useful for not only holographic and active filters, but applications involving biosensing22,23,24.

## Results and Discussion

The schematic diagram of the two types of resonators, which were fabricated at the top and the bottom layers, is presented in Fig. 1(a–c). The 0.035 mm-thick copper patterns with an electric conductivity of 5.8 × 107 S/m were made on FR-4 substrate. The 0.4 mm-thick FR-4 dielectric substrate, which has a dielectric constant of 3.9 and a loss tangent of 0.025, is used as the spacer layer. We designed the structure which included CWR with the geometrical parameters of width (w) = 2 mm and height (h) = 10 mm, and RR whose geometrical parameters were optimized to have a radius (r) = 6 mm in order to achieve the same resonance frequency with CWR and RR. The periodicity of MM was set to be 15.4 mm. A hollow tube with a radius R was used to simulate the transmission properties of bent structure, and we have fabricated a sample as shown in Fig. 1(d) and (e) to investigate the experimental transmission.

Figure 2(a) and (b) present the simulated transmission spectra of CWR alone and RR alone, respectively. The incident wave was polarized along the y direction, directly exciting the CWR and the RR. The Q-factor is evaluated by using $$Q={\omega }_{0}/{\rm{\Delta }}{\omega }_{FWHM}$$, where $${\omega }_{0}$$ is the resonance frequency and $${\rm{\Delta }}{\omega }_{FWHM}$$ is the full width at half maximum. The fundamental mode of CWR shows a low radiative loss, a narrow bandwidth and a high Q ($${{\rm{Q}}}_{1}=3.53$$). On the other hand, the RR presents a broad bandwidth and a low Q (Q2 = 1.39). The CWR exhibits a resonance at 10.1 GHz, which is higher by 0.309 GHz than that of the RR. Interestingly, when the CWR and the RR are combined as in Fig. 3(a), the interference between two eigenmodes leads to a transmission window (II) lying between two well-pronounced transmission dips (I and III). This effect is well-known to be the EIT-like effect, which originates from the bright- and bright-mode coupling. A destructive interference occurs, due to the bright- and bright-mode coupling, and this interference makes the opaque medium transparent. Each resonator exhibits resonance near 10 GHz while the transmission window appears at 5.69 GHz. To confirm this fact, we simulated the distribution of surface currents occurring in the transmission-dip region. As shown in Fig. 3(b) and (c), the surface current is formed strongly in antiparallel way for transmission dip I, but that is formed in parallel way for dip III. In the transmission dip I, a trap mode is shown, based on the magnetic resonance, which produces high Q resonance. Conversely, in transmission dip III, the radiation mode, based on the electric-resonance phenomenon, induces a broad resonance spectrum, which results in the transmission to appear at 5.69 GHz instead of 10.1 GHz.

The manifestation of EIT phenomenon depends on the difference in the phase between the two resonators in our structure. The simulated transmission spectra for MM by varying the thickness of FR4 substrate are shown in Fig. 4(a). As the thickness t s of FR4 increases, the transmission at 5.69 GHz decreases significantly. Obviously, varying the distance between the two resonators can further weaken the phase coupling strength between CWR and RR. The surface-current distribution for t s  = 0.4 mm and f = 5.69 GHz is shown in Fig. 4(b), where a strong current is generated in the CWR and the RR. On the other hand, for t s  = 4.0 mm, a weaker current distribution is observed at the CWR and the RR at 7.85 GHz, as shown in Fig. 4(c). Thus, the coupling between CWR and RR still occurs but is weakened.

We can describe the coupling effect of EIT-like transparency using the Lorentz oscillator model. In the following coupled differential equations, it is considered that both oscillators are strongly coupled to the incoming electric field $$E(t)={E}_{0}{e}^{-iwt}$$.

$$\frac{{\partial }^{2}}{\,\partial {t}^{2}}{x}_{1b}({\rm{t}})+{\gamma }_{1b}\frac{\partial }{\partial {\rm{t}}}{x}_{1b}({\rm{t}})+{\omega }_{1b\,}^{2}{x}_{1b}({\rm{t}})+{k}^{2}{x}_{2b}({\rm{t}})={E}_{1b}({\rm{t}}),$$
(1)
$$\frac{{\partial }^{2}}{\partial {t}^{2}}{x}_{2b}({\rm{t}})+{\gamma }_{2b}\frac{\partial }{\partial {\rm{t}}}{x}_{2b}({\rm{t}})+{\omega }_{2b\,}^{2}{x}_{2b}({\rm{t}})+{k}^{2}{x}_{1b}({\rm{t}})={E}_{2b}({\rm{t}}).$$
(2)

These coupled equations show that the relative coupling of incoming radiation with the two bright modes. Here, ($${x}_{1b}$$, $${x}_{2b}$$), ($${\omega }_{1b}$$, $${\omega }_{2b}$$), and ($${\gamma }_{1b}$$, $${\gamma }_{2b}$$) are the displacements, the resonance frequencies and the damping rates of two bright modes, respectively, and ($${E}_{1b,}\,{E}_{2b,}$$) are assumed to be proportional to the electric field E 0 of electromagnetic wave with proportionality constants of ($${\alpha }_{1b},\,{\alpha }_{2b}$$). k defines the coupling coefficient between two bright modes. We solve the equations by putting $${x}_{1b}(t)={N}_{1b}{e}^{-iwt}$$ and $${x}_{2b}(t)={N}_{2b}{e}^{-iwt}$$, where N is constant.

$$[\begin{array}{c}{x}_{1b}\\ {x}_{2b}\end{array}]=\frac{1}{({\omega }^{2}-{\omega }_{1b}^{2}+i\omega {\gamma }_{1b})({\omega }^{2}-{\omega }_{2b}^{2}+i\omega {\gamma }_{2b})-{k}^{4}}\times [\begin{array}{c}({\omega }^{2}-{\omega }_{2b}^{2}+i\omega {\gamma }_{2b})({E}_{1b})+{k}^{2}({E}_{2b})\\ ({\omega }^{2}-{\omega }_{1b}^{2}+i\omega {\gamma }_{1b})({E}_{2b})+{k}^{2}({E}_{1b})\end{array}].$$
(3)

The values of damping rates $${\gamma }_{1b}$$ and $${\gamma }_{2b}$$ are calculated to be 2.85 and 7.01 GHz, respectively, which are obtained from the linewidths of the curves in Fig. 2(a) and (b). The coupling coefficient k for transmission spectrum is calculated by using the formula given in refs 25 and 26, which are derived from Eq. 3. We obtained the k value at 5.65 GHz for the CWR-RR structure, resulting from the corresponding transmission peak. We can predict the EIT-like phenomena, based on the coupling between CWR and RR through this classic model.

We also investigated the capability of CWR-RR structure for the thin-film sensor, especially, in biological and biochemical fields. In order to analyze the sensitivity, the uniform dielectric overlayers were deposited on the CWR plane and the shift of resonance frequency was studied. The following three different thicknesses were performed: the CWR-RR with a overlayer of FR-4 with thickness of 10, 30 and 50 μm, as in Fig. 7. In the absence of overlayer, the resonance frequency was detected at 5.31 GHz. When the thickness of overlayer increases, the resonance frequency shifts continuously to lower frequency. The maximum shift of 711 MHz was observed for 50-μm thickness of FR-4, corresponding to a shift of 13.4% with respect to the case without overlayer. The sensitivity is defined as equation of ∆f/(nt), in which ∆f is the resonance-frequency shift, n is the refractive index, and t is the thickness27. Consequently, the sensitivity of CWR-RR is calculated as 7.2 MHz/μm. The proposed structure can achieve a larger resonance-frequency shift than the case of split-ring resonator28.

## Conclusions

This study reports the investigation of EIT-like effects at microwave frequencies, by utilizing a CWR-RR structure. We were able to implement successfully that the EIT-like effects are realized in the bilayer structure through the bright- and bright-mode coupling. It is confirmed that the transmission is manipulated by the bending parameters. In particular, at the bent state, the additional transmission peak and the wide-band transmission were observed. Our approach provides significant advance in tuning the electromagnetic response, which is useful for the potential switching sensors. In addition, our design concept might be beneficial in paving the way to thin-film sensors which are highly sensitive for biological and biochemical applications.

## Method Summary

### Electromagnetic-wave simulations

To obtain the scattering parameters of supercell, the non-periodic boundary conditions was employed in the finite-difference time-domain method by using CST Microwave Studio. For the simulation, in the tetrahedral mesh, the boundary conditions of perfect electric and magnetic conductor were assigned for the side walls (xy and x–z planes) of the 10 × 20 supercell, and the supercell was placed between two waveguide ports. The boundary along z-direction is set as open at a distance of 150 cm from the structure.

### Electromagnetic-wave transmission measurement

The transmission spectra were measured in an anechoic chamber. A Hewlett Packard E8362B network analyzer was employed, which was connected to microwave standard-gain horn antennas. The distance between two antennas was kept at 150 cm for all the measurements to minimize the near-field effects.

## References

1. Marangos, J. Electromagnetically induced transparency. J. Mod. Opt. 45, 471 (1998).

2. Phillips, D. F. et al. Storage of Light in Atomic Vapor. Phys. Rev. Lett. 86, 783 (2001).

3. Hau, L. V., Harris, S. E., Dutton, Z. & Behroozi, C. H. Light speed reduction to 17 metres per second in an ultracold atomic gas. Nature 397, 594 (1999).

4. Kuang, L. M., Chen, G. H. & Wu, Y. S. Nonlinear optical properties of an electromagnetically induced transparency medium interacting with two quantized fields. J. Opt. B: Quantum Semiclassical Opt. 5, 341 (2003).

5. Eisaman, M. et al. Electromagnetically induced transparency with tunable single-photon pulses. Nature 438, 837 (2005).

6. Chen, Y. H., Lee, M. J., Wang, I. C. & Yu, I. A. Fidelity of electromagnetically-induced-transparency-based optical memory. Phys. Rev. A 88, 023805 (2013).

7. Peng, B., Ozdemir, S.  K., Zhu, J. & Yang, L. Photonic molecules formed by coupled hybrid resonators. Opt. Lett. 37, 3435 (2012).

8. Tassin, P. et al. Planar designs for electromagnetically induced transparency in metamaterials. Opt. Express 17, 5595 (2009).

9. Gu, J. et al. Active control of electromagnetically induced transparency analogue in terahertz metamaterials. Nat. Commun. 3, 1151 (2012).

10. Shao, J. et al. Analogue of electromagnetically induced transparency by doubly degenerate modes in a U-shaped metamaterial. Appl. Phys. Lett. 102, 034106 (2013).

11. Zhang, X. et al. Electromagnetically induced absorption in a three-resonator metasurface system. Sci. Rep. 5, 10737 (2015).

12. Yang, Y., Kravchenko, I. I., Briggs, D. P. & Valentine, J. All-dielectric metasurface analogue of electromagnetically induced transparency. Nat. Commun. 5, 5753 (2014).

13. Zhang, J. et al. Electromagnetically induced transparency in metamaterials at near-infrared frequency. Opt. Express 18, 17187 (2010).

14. Zhang, F. et al. Magnetically coupled electromagnetically induced transparency analogy of dielectric metamaterial. Appl. Phys. Lett. 104, 131907 (2014).

15. Xinguang, H. et al. Plasmon induced transparency and absorption in bright–bright mode coupling metamaterials: a radiating two-oscillator model analysis. J. Phys. D: Appl. Phys. 50, 025301 (2017).

16. Jin, X.-R. et al. Manipulation of electromagnetically-induced transparency in planar metamaterials based on phase coupling. J. Appl. Phys. 111, 073101 (2012).

17. Papasimakis, N. et al. Metamaterial with polarization and direction insensitive resonant transmission response mimicking electromagnetically induced transparency. Appl. Phys. Lett. 94, 211902 (2009).

18. Bin, T., Lei, D. & Chun, J. Electromagnetically induced transparency in hybrid plasmonic-dielectric system. Opt. Express 19, 628 (2011).

19. Liao, Z. et al. Electromagnetically induced transparency metamaterial based on spoof localized surface plasmons at terahertz frequencies. Sci. Rep. 6, 27596 (2016).

20. He, X. W., Li, Y. J., Nie, M. & Wang, Q. Tunable ultrasensitive terahertz sensor based on complementary graphene metamaterials. RSC Adv. 6, 52212 (2016).

21. Nakanishi, T. & Kitano, M. ‘Implementation of Electromagnetically Induced Transparency in a Metamaterial Controlled with Auxiliary Waves. Phys. Rev. Appl. 4, 024013 (2015).

22. Genevet, P. & Capasso, F. Holographic optical metasurfaces: a review of current progress. Rep. Prog. Phys. 78, 24401 (2015).

23. Zhang, C. et al. Label-free measurements on cell apoptosis using a terahertz metamaterial-based biosensor. Appl. Phys. Lett. 108, 241105 (2016).

24. Tatara, G. et al. Proposal for an active electromagnetic metamaterial based on spin-torque oscillators. Phys. Rev. B 87, 155102 (2013).

25. Liu, N. et al. Plasmonic analogue of electromagnetically induced transparency at the Drude damping limit. Nature Mater. 8, 758 (2009).

26. Alzar, C. L. G., Martinez, M. A. G. & Nussenzveig, P. Classical analog of electromagnetically induced transparency. Am. J. Phys. 70, 37 (2002).

27. Tao, H. et al. Performance enhancement of terahertz metamaterials on ultrathin substrates for sensing application. Appl. Phys. Lett. 97, 261909 (2010).

28. Labidi, M., Tahar, J. B. & Choubani, F. Meta-materials applications in thin-film sensing and sensing liquids properties. Opt. Express 19, 733 (2011).

## Acknowledgements

This work was supported by the ICT R&D program of MSIP/IITP, Korea (2013-0-00375), and by the NRF fund by MSIP, Korea (No. 2017R1A2B4003916).

## Author information

Authors

### Contributions

J.S.H., Y.P.L., K.W.K., and L.Y.C. came up with the idea. J.S.H., Y.J.K., and Y.J.Y. conducted the fabrication and measurements. J.S.H., J.Y.R., and Y.P.L. were carried out the electromagnetic simulation and calculation. Y.P. Lee supervised the preparation of this manuscript written by J.S.H. and K.W.K. All authors discussed and commented on the manuscript. Y.P.L. supervised the project.

### Corresponding author

Correspondence to Y. P. Lee.

## Ethics declarations

### Competing Interests

The authors declare that they have no competing interests.

Publisher's note: Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.

## Rights and permissions

Reprints and Permissions

Hwang, J.S., Kim, Y.J., Yoo, Y.J. et al. Switching and extension of transmission response, based on bending metamaterials. Sci Rep 7, 3559 (2017). https://doi.org/10.1038/s41598-017-03824-4

• Accepted:

• Published:

• DOI: https://doi.org/10.1038/s41598-017-03824-4